Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites


 Valentine Thornton
 1 years ago
 Views:
Transcription
1 Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A. Aboutorabi 1 Summary The compliance equation is used to calculate the energy release rate for angle ply laminated double cantilever composite beam specimen. Instead of the traditional approach of a beam on an elastic foundation, a second order shear thickness deformation beam theory (SSTDBT) has been considered. keywords: Double Cantilever Beam, Energy Release Rate, Fracture Energy Introduction Fiberreinforced composite materials are widely used in all kinds of engineering structures owing to their high strengths and low densities. Laminated composite structures are made up of layers of orthotropic materials that are bonded together. The layers may be of different materials, or of the same orthotropic material, with the principal material directions of each layer oriented at different angles to the reference axes. By altering material or orientation, or both, of each layer, a structural designer can tailor the strength and other properties of a laminate to the requirements of a given application. Because of the low stiffness in the transverse direction, when outofplane loading exists, separation between plies occurs, i.e. delamination. The presence and growth of delamination under static or fatigue loadings will lead to safety problems by reduction of structural stiffness or initiating catastrophic fracture [1 4]. Hence in any engineering design of laminated composite structures, the delamination mode of failure should be taken into account [5,6]. Usually the delamination modes in composite laminates contain Mode I (opening), Mode II (in plane shearing) and Mode III (out of plane tearing) fractures. Therefore, it is important to characterize these fracture modes to prevent delamination damage. The overwhelming literature on delamination is mainly related to unidirectional composites. A feature that complicates the analysis of delamination growth in angle ply laminates is that delamination exists between angleplies (e.g.±θ). In an optimum laminate design, the objective will be to minimize the crack driving force and/or the crackinduced interfacial principal tensile stress in the angleply laminate under transverse shear loading. This problem is cast as a single or multicriterion optimization problem. The design variables are the ply angle θ and the relative ply thicknesses of the sublaminates. It is recognized that a delamination between angleplies has the feature of a crack between dissimilar anisotropic materials which substantially complicates the fracture mechanics analysis. 1 Faculty of Engineering, Kingston University, UK. Corresponding author:
2 62 Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 The double cantilever beam (DCB) test [7] is the most widely used method for determining the Mode I toughness of composite materials. The test specimen, the applied load, P, to the two arms and the corresponding load line displacement, δ, are schematically illustrated in Fig. 1. A model based on an EulerBernoulli beam on an elastic Winkler foundation for analysing the DCB specimen was originally developed by Kanninen [8,9] for isotropic materials and by Williams [10] for transversely isotropic materials. This model is extended to angleply laminates by Ozdil and Carlsson [11]. The beam displacements derived from this model are used to calculate the compliance and strain energy release rate of the DCB specimen. Recently, Hamed et al. [12], introduced an improved analytical model for delamination in composite beams under general edge loading which also takes into account the shearthickness deformation. In the present study, Hamed model together with the compliance equation has been used to develop a method of determining the Mode I interlaminar fracture toughness in thick angle ply laminated composites. Figure 1: Angle ply DCB specimen divided into three regions Theoretical Analysis Consider the DCB specimen in Fig. 1 made of an angle ply laminate and divided into three regions I, II and III. Assuming a second order shear thickness deformation beam theory (SSTDBT), the displacement field is u 1 (x,y,z)=u(x)+zψ x (x)+z 2 η x (x), u 2 (x,y,z)=0, (1) u 3 (x,y,z)=w(x)+zψ z (x), in all three regions, where u 1, u 2 and u 3 are the displacement components of a point in the x, y and z directions, respectively. Note that the superscripts I, II and III will be given to all of the displacement components to distinct them for the regions I, II and III. SubstitutingEq. 1 into the straindisplacement relations of elasticity we obtain ε x = ε1 0 +zκ0 1 +z 2 κ1, 1 ε y = 0, ε z = ε3, 0 γ yz = 0, γ xz = ε5 0 +zκ5 0, γ xy = 0 (2)
3 Calculation of Energy Release Rate 63 where ε 0 1 = u, κ 1 0 = ψ x, κ 1 1 = η x, ε 0 3 = ψ z, ε 0 5 = ψ x +w, κ 0 5 = 2η x +ψ z (3) and a prime denotes differentiation with respect to x. Since we are developing a beam theory, a state of plane stress is presented and therefore σ y = σ yz = 0. (4) Next by imposing Eq. 4 on three dimensional Hooke s law of elasticity, the plane stress constitutive law for the kth layer of each region is σ x σ z σ xy (k) C 11 C 13 C 16 = C 13 C 33 C 36 C 16 C 36 C 66 (k) ε x ε z γ xy (k), σ (k) xz = C (k) 55 γ (k) xz, (5) where C ij = C ij C i2c j2 i, j = 1,3,6 and C 55 = C 55 C (6) C 22 C 44 In Eq. 6, C ij denote offaxis stiffness coefficients of the kth layer [13]. Using the principle of minimum total potential energy, and considering the displacement field in Eq. 1, the equilibrium equations together with the boundary conditions (B.C. s) at boundaries and continuity conditions (C.C. s) and the equilibrium conditions (E.C. s) at the intersection of three regions will be obtained. Further by substituting the laminate constitutive relations into the equilibrium equations, the governingequilibriumequationsintermsof displacement componentsfor thethree regions will be found as A 11 u A 13 ψ z B 11 ψ x D 11 η x = 0, B 11 u B 13 ψ z D 11ψ x E 11η x +A 55(ψ x +w )+B 55 (2η x +ψ z )=0, D 11 u D 13 ψ z E 11 ψ x F 11 η x +2B 55 (ψ x +w )+2D 55 (2η x +ψ z)=0, A 55 (ψ x +w ) B 55 (2η x +ψ z )=0, A 13 u +A 33 ψ z +B 13 ψ x +D 13 η x B 55 (ψ x +w ) D 55 (2η x +ψ z )=0, (7) where A ij, B ij, D ij, E ij and F ij are laminate stiffness coefficients [12]. Giving the superscripts I, II and III to all of the displacement components and also the stiffness coefficients in Eq. 7, a system of ordinary differential equations (ODE) of order 30 will be resulted. This system of ODEs together with the B.C. s, C.C. s and E.C. s can be solved and all displacement components for thethree regions can be obtained.
4 64 Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Hamed [12] calculated the energy release rate using the Jintegral. Here the classical IrwinKies expressions [14] will be used to obtain the strain energy release rate (SERR) from the beam theory solution, i.e., G = P2 δc 2b δa. (8) where in Eq. 8, P is the load, b is the specimen width, a is the crack length and C the compliance is defined as C = δ P, (9) To obtain the G, we must first express C in terms of the crack length a. FromFig. 1, it is obvious that δ = u I 3 u II x = a 3 (10) x = a z = 0 z = 0 Because of complicated computations, however, the problem cannot be solved explicitly in terms of a. Therefore the DCB problem has been solved for a range of crack length and then a leastsquare regression was fitted to obtain C as a function of crack length, a C(a)=C 3 a 3 +C 2 a 2 +C 1 a +C 0 (11) The above equation can be differentiated with respect to crack length a and G is calculated from Eq. 8. Numerical Examples and Discussions Glass/polyester DCB specimens consisting of antisymmetric angle ply laminates of the form [±30 ] 5 and [±45 ] 5 was chosen as those in [11] where h=7.3 mm, b=20 mm, a=35 mm and l= mm. AlsoE 1 = 34.7GPa, E 2 = 8.5GPa, ν 12 = ν 13 = 0.27, ν 23 = 0.5, G 12 = G 13 = 4.34GPa, G 23 = 2.83GPa. Furtherfor θ = 45, E 3 = 9.85GPa and for θ = 30, E 3 = 9.37GPa. Considering these properties, the corresponding C i are presented in Table 1. Table 1: Polynomial coefficients of compliance in Eq. 11. Lay C 0 C 1 C 2 C 3 up [±30 ] e [±45 ] e Fig. 2a compares SERR obtained from the compliance equation with those obtained from JIntegral [12] for two antisymmetric angle ply laminates of θ = 30 and θ = 45,and for various values of crack length at constant applied load of P=40 N. The results are in good agreement with each other. In similar crack lengths,
5 Calculation of Energy Release Rate G [J/m 2 ] G [J/m 2 ] θ = 30 ο Compliance Equation θ = 45 ο Compliance Equation θ = 30 ο J Integral θ = 45 ο J Integral 50 0 q = 30 o  Compliance Equation q = 45 o  Compliance Equation q = 30 o  J Integral q = 45 o  J Integral (a) Figure 2: Comparison of pure mode I strain energy release rate, G, obtained from JIntegral and compliance equation for [±θ] 5 specimens versus (a) Crack length at constant applied load of P=40 N, (b) Applied load P at constant crack length of a=40 mm. (b) P [N] = = 45 Compliance [ m/n] SSTDBT Experiment Compliance [ m/n] SSTDBT Experiment Figure 3: Comparison of Calculated and measured Compliance = 30 = 45 G c [J/m 2 ] SSTDBT EFM G c [J/m 2 ] 200 SSTDBT EFM (a) Figure 4: Comparison of pure mode I fracture energy, G c, obtained from elastic foundation model, EFM [11] and SSTDBT using compliance equation for [±θ] 5 specimens (a) θ = 30 (b) θ = 45. SERR for θ = 45 are greater than when θ = 30. In Fig. 2b, SERR are plotted versus applied load for twoangle plylayups at constantcrack length ofa=40 mm. (b)
6 66 Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Similar to Fig. 2a, the results obtained from compliance equation are in accordance with the results from JIntegral. In Figs. 3 the calculated compliances from SSTDBT theory are compared with the experimental results obtained by Ozdil and Carlsson [11]. It is observed that when θ = 30, SSTDBT underestimates the compliance value but for θ = 45 the results are very close. In Figs. 4 pure mode I fracture energy, G c, obtained from elastic foundation model, EFM [11] and SSTDBT using compliance equation for [±θ] 5 specimens at two angleplies of θ = 30 and θ = 45 are compared. It is shown and verified that the second order shear thickness deformation beam theory (SSTDBT) together with compliance equation accurately estimates the mode I fracture toughness and strain energy release rate for any angleply laminates. The method is robust and general and other mode of fracture can be modelled using this method. References 1. Nicholls DJ, Gallagher JP. Determination of GI C in angleply composites using a cantilever beam test method. J. Reinf. Plast. Compos. 1983;2: Chai H. The characterization of mode I delamination failure in nonwoven, multidirectional laminates. Composites 1984;15: Laksimi A, Benzeggagh ML, Jing G, Hecini M, Roelandt JM. Mode I interlaminar fracture of symmetrical crossply composites. Compos. Sci. Technol. 1991;41: Robinson P, Song DQ. A modified DCB specimen for modei testing of multidirectional laminates. J. Compos. Mater. 1992;26: Johnson WS, editor. Delamination and debonding of materials, ASTM STP 876, Philadelphia, PA, Prel VJ, Davies P, Benzeggagh ML, de Charentenay FX. Mode I and Mode II delamination of thermosetting and thermoplastic composites. ASTM STP 1012, Philadelphia, PA, 1989, pp ASTM Test Method D a Mode I Interlaminar Fracture Toughness of Unidirectional Continuous Fiber Reinforced Composite Materials, Annual Book of ASTM Standards, Vol 15.03, American Society for Testing and Materials, West Conshohocken, PA. 8. Kanninen MF. An augmented double cantilever beam model for studying crack propagation and arrest. Int J Fracture 1973; 9(1): Kanninen MF. A dynamic analysis of unstable crack propagation and arrest in the DCB test specimen. Int J Fracture 1974;10(3):415.
7 Calculation of Energy Release Rate Williams JG. End corrections for orthotropic DCB specimens. Compos Sci Tech 1989;35: Ozdil F, Carlsson LA. Beam analysis of angleply laminate DCB specimens. Compos Sci Technol 1999; 59: Hamed MA, Nosier A, Farrahi GH. Separation of delamination modes in composite beams with symmetric delaminations. J. Materials & Design, 2006;27(10): Herakovich, Carl T. Mechanics of fibrous composites. NewYork: Wiley; Irwin GR, Kies JA. Critical energy release rate analysis of fracture strength. Weld J Res Suppl 1954; 33:193 8.
8
Tensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationThe Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries
The Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries M. D. Thouless Department of Mechanical Engineering Department of Materials Science & Engineering University
More informationNONLINEAR FRACTURE BEHAVIOR OF DOUBLE CANTILEVER BEAM
Engineering MECHANICS, Vol., 015, No., p. 95 10 95 NONLINEAR FRACTURE BEHAVIOR OF DOUBLE CANTILEVER BEAM Viktor Rizov* This article describes a theoretical study of nonlinear fracture behavior of the
More informationFig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double cantilever beam (DCB) specimens.
a). Cohesive Failure b). Interfacial Failure c). Oscillatory Failure d). Alternating Failure Fig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationNumerical Evaluation of Fracture in Woven Composites by Using Properties of Unidirectional Type for modelling
J. Basic. Appl. Sci. Res., 2(12)1320213209, 2012 2012, TextRoad Publication ISSN 20904304 Journal of Basic and Applied Scientific Research www.textroad.com Numerical Evaluation of Fracture in Woven Composites
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationNUMERICAL AND EXPERIMENTAL ANALYSES OF MULTIPLE DELAMINATIONS IN CURVED COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS NUMERICAL AND EXPERIMENTAL ANALYSES OF MULTIPLE DELAMINATIONS IN CURVED COMPOSITE LAMINATES A. Baldi 1 *, A. Airoldi 1, P. Belotti 1, P. Bettini
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationNumerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model
Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationMixedMode Fracture Toughness Determination USING NONCONVENTIONAL TECHNIQUES
MixedMode Fracture Toughness Determination USING NONCONVENTIONAL TECHNIQUES IDMEC Pólo FEUP DEMec  FEUP ESM Virginia Tech motivation fracture modes conventional tests [mode I] conventional tests [mode
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationExperimentally Calibrating Cohesive Zone Models for Structural Automotive Adhesives
Experimentally Calibrating Cohesive Zone Models for Structural Automotive Adhesives Mark Oliver October 19, 2016 Adhesives and Sealants Council Fall Convention contact@veryst.com www.veryst.com Outline
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationNASA TECHNICAL MEMORANDUM
NASA TECHNICAL MEMORANDUM 102777 NONLINEAR ANANLYSIS AND REDESIGN OF THE MIXEDMODE BENDING DELAMINATION TEST J. R. Reeder and J. H. Crews, Jr. January 1991 National Aeronautics and Space Administration
More informationFracture Mechanics, Damage and Fatigue Linear Elastic Fracture Mechanics  Energetic Approach
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue Linear Elastic Fracture Mechanics  Energetic Approach Ludovic Noels Computational & Multiscale Mechanics of
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationProject MMS13 Task 5 Report No 3 (M6/D3)
Project MMS13 Task 5 Report No 3 (M6/D3) Material Data Requirements and Recommended Test Methods for the Predictive Modelling of Defect Criticality in Composite Material Systems M R L Gower and G D Sims
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationEXPERIMENTBASED CRITERION FOR THE CRACK STABILITY ANALYSIS IN COMPOSITE MATERIALS
Gépészet 008 Budapest, 90.May 008. G008J04 EXPERIMENTBASED CRITERION FOR THE CRACK STABILITY ANALYSIS IN COMPOSITE MATERIALS András Szekrényes Assistant Professor, Department of Applied Mechanics,
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More informationNumerical Analysis of Delamination Behavior in Laminated Composite with Double Delaminations Embedded in Different Depth Positions
Numerical Analysis of Delamination Behavior in Laminated Composite with Double Delaminations Embedded in Different Depth Positions Numerical Analysis of Delamination Behavior in Laminated Composite with
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationSTRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES
ECCM1616 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 214 STRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES M. Nielsen a, A. T. Rhead a,
More informationID1274 SPLIT ANGLEPLY BEAM SPECIMEN FOR MEASUREMENT OF FRACTURE TOUGHNESS WITH MODE III STRESS STATE
ID1274 SPLIT ANGLEPLY BEAM SPECIMEN FOR MEASUREMENT OF FRACTURE TOUGHNESS WITH MODE III STRESS STATE Kunigal Shivakumar, Srikant Ghantae * and Matthew Sharpe Center for Composite Materials Research North
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationCharacterization of Fiber Bridging in Mode II Fracture Growth of Laminated Composite Materials
Applied Mechanics and Materials Online: 20100630 ISSN: 16627482, Vols. 2425, pp 245250 doi:10.4028/www.scientific.net/amm.2425.245 2010 Trans Tech Publications, Switzerland Characterization of Fiber
More informationSSRG International Journal of Mechanical Engineering (SSRGIJME) volume1 issue5 September 2014
Finite Element Modeling for Delamination Analysis of Double Cantilever Beam Specimen Mohammed Waseem H.S. 1, Kiran Kumar N. 2 1 Post Graduate Student, 2 Asst. Professor Dept. of Mechanical Engineering,
More informationFRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
Proc. 2 nd ESIS TC4 Conference on Polymers and Composites, in press, 1999 Author prepared reprint FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationComparison between a Cohesive Zone Model and a Continuum Damage Model in Predicting ModeI Fracture Behavior of Adhesively Bonded Joints
Copyright 2012 Tech Science Press CMES, vol.83, no.2, pp.169181, 2012 Comparison between a Cohesive Zone Model and a Continuum Damage Model in Predicting ModeI Fracture Behavior of Adhesively Bonded
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationG1RTCT A. BASIC CONCEPTS F. GUTIÉRREZSOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION
A. BASIC CONCEPTS 6 INTRODUCTION The final fracture of structural components is associated with the presence of macro or microstructural defects that affect the stress state due to the loading conditions.
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationTOUGHNESS OF PLASTICALLYDEFORMING ASYMMETRIC JOINTS. Ford Research Laboratory, Ford Motor Company, Dearborn, MI 48121, U.S.A. 1.
TOUGHNESS OF PLASTICALLYDEFORMING ASYMMETRIC JOINTS M. D. Thouless, M. S. Kafkalidis, S. M. Ward and Y. Bankowski Department of Mechanical Engineering and Applied Mechanics, University of Michigan, Ann
More informationFracture mechanics fundamentals. Stress at a notch Stress at a crack Stress intensity factors Fracture mechanics based design
Fracture mechanics fundamentals Stress at a notch Stress at a crack Stress intensity factors Fracture mechanics based design Failure modes Failure can occur in a number of modes:  plastic deformation
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationOn characterising fracture resistance in modei delamination
9 th International Congress of Croatian Society of Mechanics 1822 September 2018 Split, Croatia On characterising fracture resistance in modei delamination Leo ŠKEC *, Giulio ALFANO +, Gordan JELENIĆ
More informationMicrocracking, MicrocrackInduced. Delamination, and Longitudinal
NASA Contractor Final Report Microcracking, MicrocrackInduced Delamination, and Longitudinal Splitting of Advanced Composite Structures John A. Nairn University of Utah Salt Lake City, Utah Prepared for
More informationCHARACTERIZATION OF CURING STRESS EFFECTS ON FRACTURE BEHAVIOUR OF FRP COMPOSITE LAMINATE WITH ELLIPTICAL CUTOUTS
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS CHARACTERIZATION OF CURING STRESS EFFECTS ON FRACTURE BEHAVIOUR OF FRP COMPOSITE LAMINATE WITH ELLIPTICAL CUTOUTS Poosa R Babu, Pradhan B Department
More informationCRITERIA FOR MATRIX FAILURE IN CONTINUOUS FRPCOMPOSITES A LITERATURE STUDY. PART II: DELAMINATION
CRITERIA FOR MATRIX FAILURE IN CONTINUOUS FRPCOMPOSITES A LITERATURE STUDY. PART II: DELAMINATION Hannu Lahtinen and Juha Isometsii Rakenteiden Mekaniikka, Vol. 29 No. 1, 1996, s. 2950 ABSTRACT Some
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationSimulation of Dynamic Delamination and Mode I Energy Dissipation
Simulation of Dynamic Delamination and Mode I Energy Dissipation Muhammad Ilyas, Christine Espinosa 1, Frédéric Lachaud and Michel Salaün Université de Toulouse ISAE, DMSM, 1 Avenue Edouard Belin, 3154
More informationInt. J. Fracture, 119, 2003, 2546
Int. J. Fracture, 119, 003, 546 THE USE OF A COHESIVE ZONE MODEL TO STUDY THE FRACTURE OF FIBRE COMPOSITES AND ADHESIVELYBONDED JOINTS Blackman, B.R.K., Hadavinia, H., Kinloch, A.J. and Williams, J.G.
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationDYNAMIC DELAMINATION OF AERONAUTIC STRUCTURAL COMPOSITES BY USING COHESIVE FINITE ELEMENTS
DYNAMIC DELAMINATION OF AERONAUTIC STRUCTURAL COMPOSITES BY USING COHESIVE FINITE ELEMENTS M. Ilyas, F. Lachaud 1, Ch. Espinosa and M. Salaün Université de Toulouse, ISAE/DMSM, 1 avenue Edouard Belin,
More informationShear Lag And Beam Theories For Structures
Shear Lag And Beam Theories For Structures B N Cox, M Andrews, R Massabò, 3 A Rosakis, 4 N Sridhar, and Q D Yang Rockwell Scientific Co. LLC, Thousand Oaks, California, U.S.A. Department of Civil and Environmental
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationTESTING AND ANALYSIS OF COMPOSITE SKIN/STRINGER DEBONDING UNDER MULTIAXIAL LOADING.
TESTING AND ANALYSIS OF COMPOSITE SKIN/STRINGER DEBONDING UNDER MULTIAXIAL LOADING. Ronald Krueger*, Michael K. Cvitkovich*, T. Kevin O'Brien**, and Pierre J. Minguet*** * National Research Council Research
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More information1 Static Plastic Behaviour of Beams
1 Static Plastic Behaviour of Beams 1.1 Introduction Many ductile materials which are used in engineering practice have a considerable reserve capacity beyond the initial yield condition. The uniaxial
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationMODELING DYNAMIC FRACTURE AND DAMAGE IN A FIBERREINFORCED COMPOSITE LAMINA WITH PERIDYNAMICS
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Mechanical & Materials Engineering Faculty Publications Mechanical & Materials Engineering, Department of 011 MODELING DYNAMIC
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationDiscrete Spring Model for Predicting Delamination Growth in ZFiber Reinforced DCB Specimens
NASA/TM2004213019 ARLTR3190 Discrete Spring Model for Predicting Delamination Growth in ZFiber Reinforced DCB Specimens James G. Ratcliffe National Research Council Langley Research Center, Hampton,
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationDesign and manufacturing considerations for ply drops in composite structures
Composites: Part B 30 (1999) 523 534 Design and manufacturing considerations for ply drops in composite structures D.S. Cairns*, J.F. Mandell, M.E. Scott, J.Z. Maccagnano Montana State University, DOE
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationExamination in Damage Mechanics and Life Analysis (TMHL61) LiTH Part 1
Part 1 1. (1p) Define the Kronecker delta and explain its use. The Kronecker delta δ ij is defined as δ ij = 0 if i j 1 if i = j and it is used in tensor equations to include (δ ij = 1) or "sort out" (δ
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationExperimental characterization of interlaminar fracture toughness of composite laminates assembled with three different carbon fiber lamina
Experimental characterization of interlaminar fracture toughness of composite laminates assembled with three different carbon fiber lamina Domenico Gentile University of Cassino and Southern Lazio, Cassino
More informationPROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING. C. G. Dávila, P. P. Camanho, and M. F. de Moura
PROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING C. G. Dávila, P. P. Camanho, and M. F. de Moura Abstract The debonding of skin/stringer constructions is analyzed using a stepbystep simulation
More informationEXPERIMENTAL AND NUMERICAL INVESTIGATION ON THE FAILURE MODES OF THICK COMPOSITE LAMINATES
5 TH NTERNATONAL CONGRESS OF THE AERONAUTCAL SCENCES EXPERMENTAL AND NUMERCAL NVESTGATON ON THE FALURE MODES OF THCK COMPOSTE LAMNATES Airoldi A.*, Sala G.*, Pasqualini F.* *Aerospace Engineering Department,
More informationAN EFFICIENT SEMIANALYTICAL FINITE FRACTURE MECHANICS APPROACH FOR THE PREDICTION OF INTERLAMINAR CRACK INITIATION IN COMPOSITE LAMINATES
6th European Conference on Computational Mechanics (ECCM 6) 7th European Conference on Computational Fluid Dynamics (ECFD 7) 11 15 June 2018, Glasgow, UK AN EFFICIENT SEMIANALYTICAL FINITE FRACTURE MECHANICS
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationTensile Properties of ThermoplasticLaminated Composites Based on a Polypropylene Matrix Reinforced with Continuous Twaron Fibers
Tensile Properties of ThermoplasticLaminated Composites Based on a Polypropylene Matrix Reinforced with Continuous Twaron Fibers J. L. MENATUN, P. I. GONZALEZCHI Centro de Investigación Científica de
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationaccounts for both linear and nonlinear material response, whereas the
AN ABSTRACT OF THE THESIS OF Paul Edward Keary for the degree of Master of Science in Mechanical Engineering presented on April 26, 1984 Title: A Comparison of Experimental Mode I Analysis Methods for
More informationTentamen/Examination TMHL61
Avd Hållfasthetslära, IKP, Linköpings Universitet Tentamen/Examination TMHL61 Tentamen i Skademekanik och livslängdsanalys TMHL61 lördagen den 14/10 2000, kl 812 Solid Mechanics, IKP, Linköping University
More informationComposites: Part A 39 (2008) Contents lists available at ScienceDirect. Composites: Part A
Composites: Part A 39 (28) 1625 1631 Contents lists available at ScienceDirect Composites: Part A journal homepage: www.elsevier.com/locate/compositesa Prediction of stitch crack evolution and gas permeability
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More information